Table 83. Continued. 



Alloy 



Stress 

 (ksi) 



Percent 



Yield 



Strength 



Exposure 

 (day) 



Depth 

 (ft) 



Number of 



Specimens 



Exposed 



Number 

 Failed 



Source' 7 



5Al-2.5Sn fo 



43 



35 



197 



2,340 



3 







CEL (4) 



5Al-2.5Sn fc 



61 



50 



197 



2,340 



3 







CEL (4) 



5Al-2.5Sn fc 



92 



75 



197 



2,340 



3 







CEL (4) 



5Al-2.5Sn rf 



e 



- 



197 



2,340 



2 







CEL (4) 



5Al-2.5Sn fc 



e 



- 



402 



2,370 



2 







CEL (4) 



5Al-2.5Sn fc 



43 



35 



180 



5 



3 







CEL (4) 



5Al-2.5Sn fc 



62 



50 



180 



5 



3 







CEL (4) 



5Al-2.5Sn & 



93 



75 



180 



5 



3 







CEL (4) 



5Al-2.5Sn J 



e 



- 



181 



5 



4 







CEL (4) 



7Al-2Cb-lTa fc 



50 



50 



189 



5,900 



3 







CEL (4) 



7Al-2Cb-lTa fc ' <: 



50 



50 



189 



5,900 



3 







CEL (4) 



7Al-2Cb-lTa fc 



75 



75 



189 



5,900 



3 







CEL (4) 



7Al-2Cb-lTa fo ' r 



75 



75 



189 



5,900 



3 







CEL (4) 



7Al-2Cb-lTa fc 



35 



35 



180 



5 



3 







CEL (4) 



7Al-2Cb-lTa & 



50 



50 



180 



5 



3 







CEL (4) 



7Al-2Cb-lTa fc 



75 



75 



180 



5 



3 







CEL (4) 



7Al-2Cb-lTa d 



e 



- 



181 



5 



4 







CEL (4) 



6Al-2Cb-lTa-lMo* 



60 



50 



189 



5,900 



3 







CEL (4) 



6Al-2Cb-lTa-lMo fcc 



60 



50 



189 



5,900 



3 







CEL (4) 



eAl^Cb-lTa-lMo 6 



89 



75 



189 



5,900 



3 







CEL (4) 



6Al-2Cb-lTa-lMo fo ' c 



89 



75 



189 



5,900 



3 







CEL (4) 



6A1-4V 



48 



35 



123 



5,640 



3 







CEL (4) 



6A1-4V 6 



49 



35 



123 



5,640 



3 







CEL (4) 



6A1-4V 



68 



50 



123 



5,640 



3 







CEL (4) 



6Al-4V fe 



70 



50 



123 



5,640 



3 







CEL (4) 



6A1-4V 



102 



75 



123 



5,640 



3 







CEL (4) 



6A1-4V* 



105 



75 



123 



5,640 



3 







CEL (4) 



6Al-4V rf 



e 



- 



123 



5,640 



2 







CEL (4) 



6A1-4V 6 



66 



50 



189 



5,900 



3 







CEL (4) 



6Al-4V fr ' c 



66 



50 



189 



5,900 



3 







CEL (4) 



6Al-4V fc 



99 



75 



189 



5,900 



3 







CEL (4) 



6Al-4V fo ' c 



99 



75 



189 



5,900 



3 







CEL (4) 



6A1-4V 



43 



30 



403 



6,780 



3 







NADC (7) 



6A1-4V 



48 



35 



403 



6,780 



2 







CEL (4) 



6A1-4V* 



49 



35 



403 



6,780 



2 







CEL (4) 



6A1-4V 



71 



50 



403 



6,780 



3 







NADC (7) 



6AJ-4V 



68 



50 



403 



6,780 



2 







CEL (4) 



6Al-4V fo 



70 



50 



403 



6,780 



2 







CEL (4) 



6A1-4V 



107 



75 



403 



6,780 



3 







NADC (7) 



6AJ-4V 



102 



75 



403 



6,780 



2 







CEL (4) 



Continued 



235 



